Full Terms & Conditions of access and use can be found at
Journal of Taibah University for Science
ISSN: (Print) (Online) Journal homepage: https://www.tandfonline.com/loi/tusc20
Structural, Magnetic Properties and Electron
Paramagnetic Resonance for BaFe
Hexaferrite Nanoparticles Prepared by
M.ME. Barakat , D. El-Said Bakeer & Abdel-Hamed Sakr
To cite this article: M.ME. Barakat , D. El-Said Bakeer & Abdel-Hamed Sakr (2020) Structural, Magnetic Properties and Electron Paramagnetic Resonance for BaFe12-xHgxO19 Hexaferrite
Nanoparticles Prepared by Co-Precipitation Method, Journal of Taibah University for Science, 14:1, 640-652, DOI: 10.1080/16583655.2020.1761676
To link to this article: https://doi.org/10.1080/16583655.2020.1761676
© 2020 The Author(s). Published by Informa UK Limited, trading as Taylor & Francis Group The Authors
Published online: 12 May 2020.
Submit your article to this journal
Article views: 406
View related articles
2020, VOL. 14, NO. 1, 640–652
Structural, Magnetic Properties and Electron Paramagnetic Resonance for
Hexaferrite Nanoparticles Prepared by Co-Precipitation
M.ME. Barakat a,b, D. El-Said Bakeer c,dand Abdel-Hamed Sakr d
aPhysics Department, Faculty of Science, Taibah University, Yanbu, Saudi Arabia;bPhysics Department, Faculty of Science, Alexandria University, Alexandria, Egypt;cPhysics Department, Faculty of Science and Arts, Taibah University, Al-Ula, Saudi Arabia;dPhysics Department, Faculty of Science, Damanhour University, Damnhour, Egypt
Barium hexaferrite nanoparticles are synthesized through co-precipitation technique at different annealing temperature. Series of BaFe12−xHgxO19nanoparticles, 0.00≤ x ≤ 0.30, are prepared under the best verified conditions (annealed at 1000°C) to investigate the effect of partial substi-tution of Hg2+ions on the physical properties of BaFe12O19nanoparticles. The hysteresis loops at room temperature show the behavior of hard ferromagnetic. The estimated values of satu-ration magnetization Ms, remnant magnetization Mr and magnetic moment mBrise as Hg2+
ions content increases till x= 0.10, beyond which they reduce. A reverse trend is obtained for intrinsic coercivity Hi and coercivity Hc versus Hg2+ ions content. BaFe12−xHgxO19 nanopar-ticles are investigated through the measurements of electron paramagnetic resonance (EPR). The calculated EPR parameters show an enhancement for BaFe12−xHgxO19nanoparticles up to x= 0.10. The obtained results reveal that samples under investigation can be suitable candidate for different industrial applications.
Received 11 November 2019 Revised 17 April 2020 Accepted 21 April 2020
M-type hexagonal ferrites; XRD; TEM; EPR;
One type of magneto-plumbite group of oxides is M-type hexagonal ferrites with formula MFe12O19 (M= Ba, Sr). Specific attention for barium hexafer-rite BaFe12O19 is always increasing as a result of its large saturation magnetization, strong uniaxial mag-netic anisotropy, high Curie temperature, better coer-civity, good chemical stability and perfect corrosion resistivity, as well as its low price for production . Therefore, it plays an important role in the magnetic media as the production of permanent magnetic mate-rials, microwave devices and magnetic recording media [2–5].
The structural and magnetic properties for BaFe12 O19 can be achieved either by the substitution with different ions or by using different preparation tech-niques. The magnetic properties of barium hexaferrite can be enhanced by the partially ions substitution, espe-cially at Fe3+site either with di-, tri- or tetravalent ions [6,7]. The partial ions substitution at Fe3+site leads to change the net magnetic moment per unit and tailor magnetic properties of BaFe12O19. The enhancement of the net magnetization for this magnetic material
can be occurred when the substituted ions occupy spin down sites . Many researchers [9–12] have been investigated the impact of using the suitable tran-sition ions substation ratio at Fe site on coercivity, anisotropy and saturation magnetization for barium hexaferrite. A significant change in both magnetic and structural properties was obtained as a result of the influence of transition ions on the grains growth. On the other hand, the structural and lattice parameters, crystallite and grain sizes, as well as the dislocation density of hexaferrite samples were strongly affected by the composition and preparation conditions. Sev-eral techniques can be used for synthesizing hexafer-rites such as micro-emulsion , sol–gel [14,15], com-bustion , co-precipitation , hydro-thermal , etc. The most efficient technique for preparing hex-aferrites is co-precipitation technique due to its low cost, energy-efficient, easy method and short reaction time .
The aim of the present study is not only to obtain the optimum calcination temperature of the prepara-tion of barium hexaferrite nanoparticles by the chemical co-precipitation method but also to study the effect of
CONTACT M.ME. Barakat email@example.com
© 2020 The Author(s). Published by Informa UK Limited, trading as Taylor & Francis Group The Authors
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
Hg2+ions substitution on the structural and magnetic properties of it. In order to improve its properties to be a suitable candidate in for different industrial application.
2. Experimental techniques
2.1. Samples preparation
Barium hexaferrite nanoparticles, BaFe12O19were syn-thesized by an efficient co-precipitation technique at different annealing temperature (700, 800, 900 and 1000°C) to obtain the optimum annealing tempera-ture necessary for achieving pure phase of barium hex-aferrite. The starting materials for this synthesis are barium chloride, (BaCl2.2H2O), ferric chloride (FeCl3) and sodium hydroxide (NaOH). Stoichiometric amounts ratios of these chlorides were dissolved in distilled water, then mixed through magnetic stirrer at 60°C. An alkaline solution (NaOH) was put into the salt solution till pH was reached to 12.0. The resulting solution was heated at 90°C with continuous stirring for two hours. The precipitate was collected by magnet and washed with distilled water many times until the pH of the fil-trate reached to 7.0 in order to remove unwanted impu-rities. Then, the precipitate was dried at 80°C. Finally, the dried powders were put into a ceramic crucible and annealed at different temperatures: 700°C (B-700), 800°C (B-800), 900°C (B-900) and 1000°C (B-1000) for four hours and followed by a slow cooled to room tem-perature. Nanoparticle samples were finally ground to fine nano powder.
In order to investigate the effect of partial substitu-tion of Hg2+ions on BaFe12O19nanoparticles, a series of BaFe12−xHgxO19 nanoparticle, x= 0.00, 0.05. 0.10, 0.20 and 0.30, were synthesized through the indicated co-precipitation technique under the best verified con-ditions (annealed at 1000°C).
Phase identification of barium hexaferrite is carried out by X-ray powder diffractometer (Bruker D8 advance) with Cu-Kα radiation (λ = 1.54056 Å) in 2θ range 10–80°.
The lattice parameters a and c are determined using the following formula :
dhkl= 4(h2+ hk + k2 3a2 + l2 c2 −1/2 (1)
where dhklis the crystal face distance and (hkl) are the
The unit cell volume for barium hexaferrite can be estimated using the lattice parameters a and c from the following relation: V = √ 3 2 a 2c (2)
The theoretical (X-ray) density (ρx) and bulk density (ρb)
of the prepared powders are determined by applying Eqs.3,4, respectively. ρx = ZMwt NAV (3) ρb= m πr2h, (4)
where Z= 2 indicating 2 formula units, Mwtis material
molecular weight, m is the pellet mass, r is the pellet radius and h is the pellet thickness.
The percentage porosity (P%) of the samples is esti-mated in terms of both the theoretical and bulk densi-ties of the samples as follows :
P%= 1−ρb ρx × 100 (5)
The average nanoparticle size is determined using Jeol transmission electron microscope JEM- 2100, carried out at 200 kV through dispersing the powders in diluted HCl on a copper grid. The elemental compositions of barium hexaferrites are studied by scanning electron microscopy (SEM/ EDS; JSM-7200F). Infrared absorp-tion spectra of the samples are recorded in the range of 400–4000 cm−1 using FTIR 8400S Shimadzu spec-trophotometer. The magnetic properties of the pre-pared samples are studied by vibrating sample mag-netometer VSM, Lakeshore 7410, at room temperature. EPR spectra are measured by EPR spectrometer, Bruker Elexsys 500, at room temperature.
3. Results and discussion
In order to study the effect of annealing temperature on phase formation, the percentage, the type of impurities formed and crystallite size were determined. XRD anal-ysis was applied on the samples. Figure1shows XRD pattern of the barium hexaferrite, BaFe12O19, samples annealed at different temperatures 700°C (B-700), 800°C (B-800), 900°C (B-900) and 1000°C (B-1000). The esti-mated values of crystallite size and lattice parameters at different annealing temperature are listed in Table1. Table1clarifies that with increasing temperature, the percentage of intermediate phase Fe2O3 decreases, while the percentage of barium hexaferrite increases until reached to single phase at annealing temperature 1000°C. The crystallite size increases with increasing annealing temperature as a result of the tendency of particles, where they are collected together and form large particles. The estimated value of lattice parame-ters for samples B-700, B-800 and B-900 are inconsistent with the reported values as a result of the presence of impurities beside the basic phase. On the other hand, the lattice parameters for sample B-1000 are consistent with published values [22,23].
Figure2shows XRD patterns of hexaferrite BaFe12−x HgxO19 nanoparticles annealed at 1000°C for 4 h,
Figure 1.XRD patterns of BaFe12O19nanoparticles annealed at diﬀerent temperatures.
Table 1.Barium hexaferrite and intermediate impurity phase percentages, lattice constants and average crystallite size for BaFe12O19 nanoparticles prepared at diﬀerent annealing
temperature. Sample BaFe12O19(%) Fe2O3(%) a (Å) c (Å) L (nm) B-700 69.7 31.3 5.870 23.239 32.88 B-800 82.2 17.8 5.875 23.206 34.76 B-900 91.0 9.0 5.809 23.234 35.45 B-1000 100 0.0 5.893 23.132 36.08
Figure 2.XRD patterns of BaFe12−xHgxO19 nanoparticles
annealed at 1000°C for 4 h.
x= 0.00, 0.05, 0.10, 0.20 and 0.30. All diffraction peaks in the pattern were belonging to those of M-type bar-ium hexaferrite BaFe12O19with space group P63/mmc (194) from JCPDS card number 01-084-0757. From the diffraction patterns, they show the crystallite as sin-gle phase of the prepared samples, with no impurity phases. The calculated lattice parameters for undoped
sample, a= 5.893 Å and c = 23.132 Å, are consistent with JCPDS card number 01-084-0757 . Figure 3
shows the lattice parameters variation versus x. It is seen that the lattice parameter c increases with increasing x, while the lattice parameter a slightly decreases. The increase in c can be attributed to the partial substitu-tion of the smaller ionic radius Fe3+ ions (0.64 Å) by larger ionic radius Hg2+ions (1.02 Å). More variation is observed for lattice parameter c because of c-axis is easy axis which the spins can freely rotate around this axis, comparing with a-axis. The ratio c/a has been calcu-lated for all the prepared samples and found to be in the range 3.925–3.983, confirming with Vegard’s law as the ratio c/a should be less than 3.98 for M-type hex-aferrite . Moreover, the unit cell volume decreases from 695.688 Å3 for x= 0.00–688.106 Å3 for x= 0.30 (Table2). This decrease is due to the strongly depen-dence of unit cell volume on a (V α a2) more than c. The calculated values of X-ray density (ρx), bulk density
(ρb) and percentage of porosity (P%) are listed in Table2
versus Hg+2ions content. It is displayed the increase of (ρx) and (ρb) with increasing x, which is attributed to the
larger atomic weight and density of Hg 200.59 g mol−1 and 13.56 g cm−3, respectively, comparing with Fe of
Figure 3.The variation of the lattice parameters a and c versus Hg2+ions content.
density 7.87 g cm−3and atomic weight 55.84 g mol−1. It is observed thatρxis higher thanρbdue to the presence
of pores which affected by sintering temperature  and the syntheses conditions . The results showed that porosity follows the inverse behaviour ofρx, it is
found to increase as the Hg2+ion content increases. The increase in porosity may be attributed to the diminu-tion of oxygen vacancies or the formadiminu-tion of a solid solution .
The average crystallite size (L) for the prepared
sam-ples is estimated by taking the average value of the most intense diffraction peaks using the Debye Scherrer formula  and their values are tabulated in Table2. The average crystallite size is calculated from Scherer equation and is found to increase from 36.077 nm at x= 0.00 to 37.544 nm at x = 0.10 and then it decreases to minimum value 26.971 nm at x= 0.30. The decreas-ing trend of crystallite size may be due to the high concentration of Hg2+ions content which reduces the grain growth because of isolation on or close to the grain boundary which impedes its movement.
The morphologies of hexaferrite BaFe12−xHgxO19 nanoparticles are shown in Figure 4. It is clear that the samples are composed of approximately lamel-lar grains. There are agglomerations between the par-ticles which may be due to the high magnetization and the magnetic interaction between the particles  or related to particles chemical reaction at the time of calcination procedure. The particle size (w) of BaFe12−xHgxO19 nanoparticles obtained at 1000°C, is mainly between 41.86 and 53.29 nm. Table 2 shows
that the values of w are slightly higher than those obtained from XRD (L). This is because of X-rays can detect the individual crystallite parts into the nanopar-ticle, as TEM deals with the grain which might consist of a number of crystallites. As present in Table2, it is clear that w has the same behaviour of L with Hg2+ions content.
The elemental analysis of BaFe12−xHgxO19 nanopar-ticles is investigated by Energy dispersive X-ray analy-sis (EDS). The results indicate the presence of Ba, Fe, Hg, and O peaks as seen in Figure 5, affirming the formation of BaFe12−xHgxO19solid solution and indi-cates Hg2+ ions incorporation in the BaFe12O19 host lattice. Experimental and theoretical atomic percent-ages (%) of BaFe12−xHgxO19 nanoparticles, x = 0.00, 0.10 and 0.30, are inserted in the EDS Figs. It is clear the rapprochement between the calculated and exper-imental values of the atomic percentages for all ele-ments. FTIR absorption spectra of M-type hexaferrite BaFe12−xHgxO19 nanoparticles recorded in range of 400–4000 cm−1 are seen in Figure 6(a). Two main absorption bands υ1 and υ2 in the ranges 560– 590 cm−1 and 430–450 cm−1 are observed which are characteristic to M-type barium hexaferrite. The band υ1is attributed to the stretching vibrations of the tetra-hedral A-site andυ2to the octahedral B-site vibrations . It is observed that the values ofυ1are higher than υ2, indicating that the vibration normal mode for A-sites is larger than that of B-sites. This is attributed to shorter bond length of the A-site clusters than that of the B-site clusters . Also, the bandυAshows up in the spectra
Table 2.XRD parameters of BaFe12−xHgxO19nanoparticles annealed at 1000°C for 4 h.
Hg2+ions content (x) a (Å) c (Å) c/a V(Å3) ρx(g/cm3) ρb(g/cm3) P% L (nm) w (nm)
0.00 5.893 23.132 3.925 695.688 5.31 3.76 28.94 36.077 46.955
0.05 5.883 23.138 3.933 693.512 5.36 3.89 27.20 37.294 48.835
0.10 5.876 23.239 3.955 694.883 5.38 4.08 24.14 37.544 53.296
0.20 5.860 23.257 3.969 691.639 5.48 4.35 20.47 32.784 47.921
0.30 5.852 23.261 3.974 689.871 5.56 4.67 15.82 26.971 41.860
Figure 4.TEM images of BaFe12−xHgxO19nanoparticles. at around 880 cm−1and is attributed to increment in the concentration of divalent ions among the A-sites . The appearance of this band confirms the repre-sents the divalent metal- oxygen vibrations and may
assign to the existence of Hg2+– O2−or/and Fe2+– O2− among A-sites. Carbonyl group (C= O) with asymmet-ric stretching is detected at 1633 cm−1. The detection of band around 3438 cm−1is assigned to the O–H bond
Figure 7.Room temperature magnetic hysteresis loops of BaFe12−xHgxO19nanoparticles, x= 0.00, 0.05, 0.10, 0.20 and
of water with stretching vibration which represents the appearance of hydrogen-bonded chains .
The thermal properties of M-type hexaferrite can be discussed in terms of mean value of wave numberυav of the characteristic peaks υ1 and υ2 as follows , and their values are listed in Table3versus Hg+2ions content.
where TD is Debye temperature in Kelvin andis the
velocity of light.
The variation of TDversus Hg2+ions content is shown
in Figure6(b). It is demonstrated that TD values show
increment behaviour against x. The variation of TD is
attributed to the variation of the mean value of the char-acteristic wave numberυavof IR bands . For n-type materials, according to specific heat theory, the conduc-tion electrons can absorb part of the heat resulting in a decrease in Debye temperature. And therefore, the increasing trend of TD confirms the reduction of
con-duction electrons (i.e.n-type) and increment of the holes contribution (i.e.p-type) by increasing Hg2+ions .
The magnetic hysteresis loops, at room tempera-ture for BaFe12−xHgxO19 nanoparticles are shown in Figure7. The magnetic measurements are carried out under an applied field of±20 kG. It is displayed wide hysteretic behaviour curves (large coercivity Hc) which
distinguish the hard magnetic materials [35,36]. The sat-uration magnetization values (Ms) are estimated from
the approximation of Stoner-Wohlfarth (S-W) using the following equation : M= Ms 1− α H2 (7)
According to eq. (7), the plot of M versus 1/H2(Figure8) leads to a straight line with slope= Ms× α. The
inter-section of this straight line with y-axis gives the values of saturation magnetization Ms. The estimated values
of Msandα are displayed in Table4versus Hg+2ions
content. It is observed that Msand remnant
magnetiza-tion Mrrise with increasing x and attained the maximum
value at x= 0.10, beyond which they decrease. The increase in Msis mainly attributed to the strengthening
of super-exchange interactions among nanoparticles due to the partial substitution of Fe3+ions by the Hg2+ ions. The ions radii Hg2+ions (1.02 Å) is larger than that Fe3+ions (0.64 Å). This leads to decrease the different magnetic ions distances and subsequently enhance the strength of the super-exchange interactions . On the other hand, the Fe3+ions in barium hexaferrite have five sites are up-spins (↑), whereas two sites are down-spins (↓) . The increase in Ms is attributed to the
occu-pation of Hg2+ ions in the down-spin states. The net spin in upward direction consequently increases, lead-ing to enhance Msup to x= 0.10. While the decreasing
Figure 8.The plots of M versus 1/H2for BaFe
12−xHgxO19nanoparticles. Table 3.The distinguishing wave number υ1, υ2
corre-sponding to diﬀerent vibrations and Debye temperature of BaFe12−xHgxO19nanoparticles. Hg2+ions content (x) υ1(cm−1) υ2(cm−1) υav(cm−1) TD(K) 0.00 590.307 438.362 514.335 739.613 0.05 591.834 443.095 517.465 744.114 0.10 592.052 444.524 518.288 745.298 0.20 593.012 445.116 519.064 746.414 0.30 593.893 446.208 520.051 747.833
from the enhancement of nonmagnetic Hg2+ions con-centration and existing of spin canting due to magnetic collinearity loss.
The magnetic moment (mB) per formula unit in Bohr
magneton (μB) can be calculated through the following equation :
5585 , (8)
where Mw is the molecular weight of each
composi-tion. The obtained values of magnetic moment are pre-sented in Table4versus x. It is observed that mB has
the same trend with x as Ms. The increase in the
crys-tallite size L and the decrease in spin canting angle lead to enhance Ms, mBand the strength of A–B
super-exchange magnetic interactions .
The magneto crystalline anisotropy constant (Kmag)
and the intrinsic coercivity (Hi) can be deduced from the
following relations [40,41]: Kmag= Ms 15α 4 0.5 (9) Hi= 2Kmag Ms (10)
The estimated values of Kmag and Hi are also
pre-sented in Table4versus x. It is obvious that Hislightly
decreases as Hg2+ions content increases till x= 0.10, and then increases with further increase in x, and become close to that of x= 0.00. The reduction in Hi may be attributed to the non-magnetic Hg2+ ions
which make the inter-sublattice interactions weak, lead-ing to decrease the anisotropy energy and Hi .
CoercivityHcalso decreases from 4943 G at x= 0.00 to
4345 G at x= 0.10 and then rises to 4900 at x = 0.30. The variation of Hc is associated with the extrinsic
effect which related to porosity and the distribution of grain size, as well as the intrinsic effect which directly related to the anisotropy field . From the results listed in Table2, it is observed that Hcdecreases with
increasing the grain size and with decreasing the poros-ity which improves the inter grain connectivporos-ity across the crystal lattice. The other reason of the decrease in Hc may be ascribed to the decrease in magneto
crystalline anisotropy. Frequently, we can use the vari-ations in Hi values to explain the Hc variations .
The high values of Hi indicate the hard magnetic
behaviour of the samples. Figure 9 shows that Hi of
the samples is proportional to Hc and depends on
crystallite size. Usually, the values range of coercivity determines the application in which nanomaterials are used, for example the substances that have Hc< 1200 G
is applicable in the field of perpendicular magnetic recording media . Moreover, as-prepared hexafer-rites nanoparticles of Hc in the range (4943–4345 G)
with Hc > Mr/2, are known as permanent magnets
which have a potential candidate for numerous appli-cations.
Table 4.Magnetic parameters of BaFe12−xHgxO19nanoparticles.
Hg2+ions content (x) Ms(emu/g) Mr(emu/g) Hc(G) mB(μB) Kmag(erg/G) Hi(G)
0.00 56.38 25.254 4943 11.22 448167.10 15898.09
0.05 57.93 26.529 4682 11.60 442169.37 15265.64
0.10 62.37 30.647 4345 12.57 440594.50 14128.64
0.20 59.99 28.707 4645 12.25 474298.17 15812.84
0.30 59.91 28.306 4900 12.34 497120.46 16595.58
Figure 9.The variation of Hcand Hiwith the crystallite size L.
Figure 10.First-derivative absorption spectra for BaFe12−xHgxO19nanoparticles versus the magnetic ﬁeld. The study of EPR of ferrites is very important for
investigation high frequency magnetic properties as the resonance originates from the spins-electromagne tic waves interaction . Figure10 shows the first-derivative electron paramagnetic resonance absorp-tion spectra at room temperature for BaFe12−xHgxO19
samples with 0.00≤ x ≤ 0.30. EPR spectra contain an isotropic with relative narrow EPR line, characterizing Ba ferrite samples . The isotropic behaviour of EPR line, for all substituted samples, reflects its symmetry about the central position. This indicates the absence of skin effect . In ferrites, Fe3+ions are the main responsible
for EPR spectra as EPR signal for Fe2+ions can be only observed at very low temperature (∼ 4 K) because of their very short spin–lattice relaxation time . On the other hand, the two main sources which are responsi-ble for the EPR signal linewidth for any ferrite material are the interaction between magnetic dipoles among particles and the super-exchange interactions between magnetic ions through the ions of oxygen .
The strong EPR intensity display slightly shift for the point of maximum derivative with increasing Hg substitution. This makes a slight change in g-factor. The g-factor was calculated from knowing the g-factor of CuSO4.5H2O . The g-factor variation with x for BaFe12−xHgxO19 samples is shown in Figure 11. The g-factor is near ≈ 2, corresponding to barium ferrite sample . There is a slight increase in g-factor with increasing Hg2+ions content up to x= 0.10, followed by a decrease with further increase in x. The slight reduc-tion of g-factor for x≥ 0.20 reflect the decrease in the magnetic interaction. Reverse behaviour for the reso-nance field Hrversus x is plotted in Figure11. The EPR line intensity of peak-to-peak amplitude Y* increases with increasing Hg substitution up to 0.10, beyond which it decreases as represented in Figure 11. This enhancement indicates the enhancement of unpaired electrons in BaFe12−xHgxO19 samples. Moreover, the variation of peak-to-peak line width xpp with Hg2+ ions content is also shown in Figure11. It is clear that xpp increases with increasing Hg2+ ions content up to x= 0.10, beyond which it decreases. The increase inxppreflects the strengthening of the dipolar inter-action and indicates the existence of critical grain size with 0.00≤ x ≤ 0.10 as the crystalline size increases up to x= 0.10. On the other hand, the decrease in xppfor x≥ 0.20 can be interpreted as the reduction of magnetic interaction effect, according to the reduc-tion of magnetic ions (Fe3+ions), confirming with the model of solid solutions with magnetic dilution;xpp∝ (1 − x)1/2. The number of spins N participating in
the resonance are estimated from comparing the area under the absorption curve with that for CuSO4.5H2O . N enhances as Hg2+ ions content increases up to x= 0.10, beyond which it decreases as listed in Table 5. This enhancement of N, as well as g-factor andxppreflects the increase of the crystalline degree for BaFe12−xHgxO19samples as x increases up to 0.10, which improve the dipole interaction that in turn give largexpp, g-factor and N . The paramagnetic sus-ceptibilityχ at room temperature is calculated through the following relation :
χ = Ng2μ2
BJ(J + 1)/3kBT (11)
where μB is Bohr magneton and J is total angular
momentum. The values of paramagnetic susceptibility versus Hg2+ions content are listed in Table5. It is clear thatχ increases with increasing x up to 0.10, confirming
Figure 11.The variation of g-factor, Hr,xppand Y* versus x
Table 5.Variation of N,χ and τ versus x for BaFe12−xHgxO19
nanoparticles. x N× 1022(spin/g) χ × 10−3(emu/g) τ × 10−9(s) 0.00 1.94 5.01 1.30 0.05 3.14 8.26 1.26 0.10 4.15 11.14 1.21 0.20 2.41 6.30 1.36 0.30 1.57 3.97 1.43
with the behaviour of N with x. The order of param-agnetic susceptibility is comparable with that obtained for BaFe12O19sample . The spin relaxation process is characterized by a time constant that is a function of magnetic field. It depends on the rate at which the energy of microwave can be emitted or absorbed to the surrounding spins. The spin–spin relaxation time con-stant T can be calculated through the following relation : 1 T = gβx1/2 -h ,x1/2 = √ 3xpp (12) where β is Bohr magneton, x1/2 is the linewidth at half height of absorption peak. The values of spin–spin
relaxation time constant versus Hg2+ions content for BaFe12−xHgxO19samples are also listed in Table5. One can notice that T decreases with increasing Hg2+ions content up to x= 0.10, followed by a decrease for fur-ther increase in x. The behaviour could be explained according to the change in electron motion and the strength of super-exchange interaction between mag-netic ions through oxygen.
Barium hexaferrite nanoparticles were prepared at dif-ferent temperature through a co-precipitation method. XRD diffraction patterns revealed that the annealing temperature played an important role in the crystalliza-tion of barium hexaferrite. A series of BaFe12−xHgxO19 nanoparticle, 0.00 ≤ x ≤ 0.30 were successfully pre-pared at the optimum annealing temperature 1000°C. XRD and FTIR analysis confirmed the single phase for-mation and the absence of impurities. Lattice param-eter c increased with the increase in x, whereas a slightly decreased. M-H curves displayed wide hys-teretic behaviours with higher coercivity which is char-acteristic of the typical hard magnetic materials, lead-ing to recommend these materials to be a potential candidate for numerous applications such as recording media applications. M-H curves indicated the enhance-ment in saturation magnetization values (Ms) and
rem-nant magnetization Mr up to x= 0.10 followed by
a decrease up to x= 0.30. On the other hand the intrinsic coercivity (Hi) and coercivity Hcdiminished as
Hg2+content increased till x= 0.10, beyond which they enhanced. The decrease in Hcmight be ascribed to the
increase in the grain size and the decrease in magneto crystalline anisotropy. The increase of Hg2+ content up to 0.10 for BaFe12−xHgxO19nanoparticle improved the dipole interaction that in turn made an enhance-ment for the values of g-factor, peak-to-peak line width, number of spin and paramagnetic susceptibility. The enhancement of these EPR parameters confirmed the improvement of the crystalline degree as Hg2+content increased up to 0.10, reflecting the existence of critical grain size with 0.00≤ x ≤ 0.10.
No potential conflict of interest was reported by the author(s).
M.ME. Barakat http://orcid.org/0000-0003-3730-3710
D. El-Said Bakeer http://orcid.org/0000-0002-8456-5134
Abdel-Hamed Sakr http://orcid.org/0000-0003-0095-5774
 Mosleh Z, Kameli P, Ranjbar M, et al. Effect of
anneal-ing temperature on structural and magnetic proper-ties of BaFe12O19 hexaferrite nanoparticles. Ceram Int
 Pullar RC. Hexagonal ferrites: A review of the synthesis, properties and applications of hexaferrite ceramics. Prog Mater Sci.2012;57(7):1191–1334.
 Harris VG, Geiler A, Chen Y, et al. Recent advances in pro-cessing and applications of microwave ferrites. J Magn Magn Mater2009;321:2035–2047.
 Chen D, Liu Y, Li Y, et al. Microstructure and magnetic properties of Al-doped barium ferrite with sodium cit-rate as chelate agent. J Magn Magn Mater 2013 ;337-338:65–69.
 Almessiere MA, Slimani Y, El Sayed HS, et al. Investi-gation of Microstructural and magnetic properties of BaVxFe12−xO19 Nanohexaferrites. J Supercond Nov Magn.2019;32:1437–1445.
 Maria Lumina Sonia M, Anand S, Maria Vinosel V, et al Effect of lattice strain on structure, morphology and magneto-dielectric properties of spinel NiGd x Fe 2−x O 4 ferrite nano-crystallites synthesized by sol-gel route. J Magn Magn Mater2018;466:238–251.
 Elayakumar K, Dinesh A, Manikandan A, et al. Struc-tural, morphological, enhanced magnetic properties and antibacterial bio-medical activity of rare earth element (REE) cerium (Ce3+) doped CoFe2O4 nanoparticles. J Magn Magn Mater.2019;476:157–165.
 Rai GM, Iqbal MA, Kubra KT. Effect of Ho3+ substi-tutions on the structural and magnetic properties of BaFe12O19 hexaferrites. J Alloy Compd.2010;495:229– 233.
 Chen W, Wu W, Mao M, et al. Improvement of the mag-netization of barium hexaferrites Induced by substitution of Nd3+ ions for Fe3+ ions. J Supercond Nov Magn.
 Slimani Y, Baykal A, Manikandan A. Effect of Cr 3+ sub-stitution on AC susceptibility of Ba hexaferrite nanoparti-cles. J Magn Magn Mater2018;458:204–212.
 Topkaya R. Effect of Zn substitution on temperature dependent magnetic properties of BaFe12O19 hexafer-rites. J Alloy Compd.2017;725:1230–1237.
 Amer MA, Meaz TM, Attalah SS, et al. Structural and magnetic studies of Ti4+substituted M-type BaFe12O19 hexa-nanoferrites. Mater Sci Semicond Process2015;40: 374–382.
 Ali I, Islam MU, Ashiq MN, et al. Investigation of the magnetic properties of nanometric SrSmCoNi ferrite/PST matri. Ceram Int.2015;41:8748–8754.
 Kaur T, Kaur B, Bhat BH, et al. Effect of calcination temper-ature on microstructure, dielectric, magnetic and opti-cal properties of Ba0.7La0.3Fe11.7Co0.3O19 hexaferrites. Physica B.2015;456:206–212.
 Khan HM, Islam MU, Xu Y, et al. Structural and mag-netic properties of TbZn-substituted calcium barium M-type nano-structured hexa-ferrites. J Alloys Compd
 Sharma R, Agarwala RC, Agarwala V. A study on the heat-treatments of nanocrystalline nickel substituted BaW hexaferrite produced by low combustion synthesis method. J Magn Magn Mater.2007;312:117.
 Yu H. Bafe12o19 powder with high magnetization pre-pared by acetone-aided coprecipitation. J Magn Magn Mater.2013;341:79–85.
 Tang X, Hong RY, Feng WG, et al. Ethylene glycol assisted hydrothermal synthesis of strontium hexafer-rite nanoparticles as precursor of magnetic fluid. J Alloys Compd2013;562:211–218.
 Ghoneim AI, Amer MA, Meaz TM, et al. Dielectric proper-ties of Ti4+ substituted BaFe12O19 nanoparticles. Phys-ica B.2017;507:1–12.
 Catellanos PAM, Jarque JCS, Rivera JA. Magnetic and microstructural properties of the BaFe(12−(4/3)x)Snx O19 ceramic system. Physica B.2005;362:95–102.  Safaan SA, Abo El Ata AM, El Messeery MS. Study
of some structural and magnetic properties of Mn-substituted SrCu hexagonal ferrites. J Magn Magn Mater
 Kumar S, Manglam MK, Supriya S, et al. Lattice strain mediated dielectric and magnetic properties in La doped barium hexaferrite. J Magn Magn Mater.2019;473:312– 319.
 Kaur P, Chawla SK, Narang SB, et al. Effect of Cu-Co-Zr Doping on the properties of Strontium hexaferrites syn-thesized by Sol-Gel Auto-combustion method. J Super-cond Nov Magn.2017;30:635–645.
 Almessiere MA, Slimani Y, Tashkandi NA, et al. The effect of Nb substitution on magnetic properties of BaFe12O19 nanohexaferrites. Ceram Int2019;45:1691–1697.  Islam MU, Ahmad I, Abbas T, et al. pp. 19–23, 155–158.
Proceedings of 6th International Symposium on Advan ced Materials, Islamabad (1999).
 Deraz NM, Alarif A. Int J Electrochem Sci2012;7:4585.  Verma A, Thakur OP, Prakash C, et al. Temperature
depen-dence of electrical properties of nickel–zinc ferrites pro-cessed by the citrate precursor technique. Mater Sci Eng B.2005;116:1–6.
 Cullity BD. Powder photographs, Debye Scherrer Method, 150–151, Elem. of X-ray Diffr., Addision Wesley Publishing Companym Inc., Reading, Massachusetts, M. Cohen, Printed in U.S.A; 1956.
 Kumar ER, Jayaprakash R, Kumar S. The role of anneal-ing temperature and bio template (egg white) on the structural, morphological and magnetic proper-ties of manganese substituted MFe2O4 (M= Zn, Cu, Ni, Co) nanoparticles. J Magn Magn Mater 2014;351: 70–75.
 Amer MA, Meaz TM, Mostafa AG, et al. Time effect of annealing on phase transformations of Cu–Al–Cr nano-ferrites prepared by a co-precipitation method. Mater Sci Semicond Process2015;32:68–75.
 Singh J, Singh C, Kaur D, et al. Elucidation of phase evo-lution, microstructural, mössbauer and magnetic prop-erties of Co2+Al3+ doped M-type Ba Sr hexaferrites synthesized by a ceramic method. J Alloys Compd
 Patange SM, Shirsath SE, Lohar KS, et al. Infrared spec-tral and elastic moduli study of NiFe2−xCrxO4 nanocrys-talline ferrites. J Magn Magn Mater2013;325:107–111.  Patange SM, Shirsath SE, Jadhav SP, et al. Elastic
proper-ties of nanocrystalline aluminum substituted nickel fer-rites prepared by co-precipitation method. J Mol Struct
 Mazen SA, Mansour SF, Dhahri E, et al. The infrared absorption and dielectric properties of Li–Ga ferrite. J Alloy Compd.2009;470:294–300.
 El-Sayed SM, Meaz TM, Amer MA, et al. Magnetic behavior and dielectric properties of aluminum substi-tuted M-type barium hexaferrite. Physica B. 2013;426: 137–143.
 Teh GB, Nagalingam S, Jefferson DA. Preparation and studies of Co(II) and Co(III)-substituted barium
ferrite prepared by sol–gel method. Mater Chem Phys
 Amir M, Gungunes H, Slimani Y, et al. Mössbauer Studies and magnetic properties of Cubic CuFe2O4 nanoparti-cles. J Supercond Nov Magn.2019;32:557–564.
 Almessiere MA, Slimani Y, Baykal A. Structural and magnetic properties of Ce-doped strontium hexaferrite. Ceram Int2018;44:9000–9008.
 Bobade DH, Rathod SM, Mane ML. Sol–gel auto-combus tion synthesis, structural and enhanced magnetic prop-erties of Ni2+ substituted nanocrystalline Mg–Zn spinel ferrite. Physica B.2012;407:3700–3704.
 Slimani Y, Baykal A, Amir M, et al. Substitution effect of Cr3+ on hyperfine interactions, magnetic and optical properties of Sr-hexaferrites. Ceram Int2018;44:15995– 16004.
 Almessiere MA, Slimani Y, Baykal A. Structural, morpho-logical and magnetic properties of hard/soft SrFe12-xVxO19/(Ni0.5Mn0.5Fe2O4)y nanocomposites: effect of vanadium substitution. J Alloy Compd. 2018;767:966– 975.
 Ali I, Islam MU, Awan MS, et al. Effect of Tb3+ substitution on the structural and magnetic properties of M-type hex-aferrites synthesized by sol–gel auto-combustion tech-nique. J Alloys Compd2013;550:564–572.
 Slimani Y, Güngüneş H, Nawaz M, et al. Magneto-optical and microstructural properties of spinel cubic copper ferrites with Li-Al co-substitution. Ceram Int
 Ali I, Islam MU, Awan MS, et al. Effects of Ga–Cr substitu-tion on structural and magnetic properties of hexaferrite (BaFe12O19) synthesized by sol–gel auto-combustion route. J Alloys Compd2013;547:118–125.
 Gazeau F, Bacri JC, Gendron F, et al. Magnetic res-onance of ferrite nanoparticles. J Magn Magn Mater
 Koksharov YA, Pankratov DA, Gubin SP, et al. Electron paramagnetic resonance of ferrite nanoparticles. J Appl Phys2001;89:2293–2298.
 Bejjit L, Haddad M. EPR study, in the normal and super-conducting states, of GdBa2Cu3O7 single crystal before and after grinding. Physica C.2002;371:339–343.  Sastry MD, Nagar YC, Bhushan B, et al. An unusual
radiation dose dependent EPR line at geff = 2.54 in feldspars: possible evidence of Fe3+O2−↔ Fe2+O−and exchange coupled Fe3+–Fe2+–nO−. J Phys Condens Matter.2008;20:025224.
 Singh JP, Dixit G, Srivastava RC, et al. Magnetic reso-nance in superparamagnetic zinc ferrite. Bull Mater Sci
 Weil JA, Bolton JR. Electron paramagnetic resonance – Elementary theory and Practical applications. 2nd ed. Hoboken (New Jersey): John Wiley & Sons, Inc.;2007.  Mendoza A, Prado J, Almanza O. Structural and magnetic
Features of Mn1−xZnxFe2O4nanoparticles. Acta Phys Pol A.2012;121:950–953.
 Li X, Lu G, Li S. Synthesis and characterization of fine par-ticle ZnFe2O4 powders by a low temperature method. J Alloys Compd.1996;235:150–155.
 Aschcroft NW, Mermin ND. Solid State Physics. New York: Harcourt College Publishers;2001.
 Shahane GS, Kumar A, Arora M, et al. Synthesis and char-acterization of Ni–Zn ferrite nanoparticles. J Magn Magn Mater2010;322:1015–1019.